#------------------------------------------------------------------------------
#$Date: 2016-02-16 03:10:39 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176453 $
#$URL: svn://www.crystallography.net/cod/cif/7/10/72/7107295.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7107295
loop_
_publ_author_name
'Wendy L. Queen'
'J. Palmer West'
'Shiou-Jyh Hwu'
'Thanh Thao Tran'
'P. Shiv Halasyamani'
'Don VanDerveer'
_publ_section_title
;
 Symmetry preservation in a new noncentrosymmetric lattice comprised of
 acentric POM clusters residing in bowls of Cs+ -based half SOD B-cage
;
_journal_name_full               Chem.Commun.
_journal_page_first              1665
_journal_paper_doi               10.1039/c1cc16264k
_journal_volume                  48
_journal_year                    2012
_chemical_formula_sum            'As8 Br Cs5 O43.5 V14'
_chemical_formula_weight         2752.97
_chemical_name_systematic
;
?
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 98.98(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   13.454(5)
_cell_length_b                   19.222(4)
_cell_length_c                   22.564(4)
_cell_measurement_reflns_used    5052
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.05
_cell_measurement_theta_min      1.97
_cell_volume                     5764(3)
_computing_cell_refinement       'CrystalClear (Rigaku/MSC, 1999)'
_computing_data_collection       'CrystalClear (Rigaku/MSC, 1999)'
_computing_data_reduction        'CrystalClear (Rigaku/MSC, 1999)'
_computing_molecular_graphics    'SHELXL-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 14.6199
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_details
;
scan:
Number of images: 260
Slice: -40.0000 - 90.0000
Image width: 0.5000
Exp time: 120.0000
Rotation axis: Omega
Omega: 0.0000
Chi: 45.0000
Phi: 0.0000
XTD: 27.7265
2theta: 0.6262
scan:
Number of images: 89
Slice: -30.0000 - 14.5000
Image width: 0.5000
Exp time: 120.0000
Rotation axis: Omega
Omega: 0.0000
Chi: 45.0000
Phi: 90.0000
XTD: 27.7265
2theta: 0.6262
;
_diffrn_measurement_device_type  'Rigaku AFC8S'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1527
_diffrn_reflns_av_sigmaI/netI    0.1313
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            17539
_diffrn_reflns_theta_full        25.05
_diffrn_reflns_theta_max         25.05
_diffrn_reflns_theta_min         1.97
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    10.609
_exptl_absorpt_correction_T_max  0.8158
_exptl_absorpt_correction_T_min  0.4168
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'REQAB, CrystalClear'
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    3.172
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       column
_exptl_crystal_F_000             4975
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.02
_refine_diff_density_max         1.795
_refine_diff_density_min         -1.308
_refine_diff_density_rms         0.321
_refine_ls_extinction_coef       0
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.077
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     364
_refine_ls_number_reflns         5052
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.077
_refine_ls_R_factor_all          0.1632
_refine_ls_R_factor_gt           0.0862
_refine_ls_shift/su_max          0.052
_refine_ls_shift/su_mean         0.003
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1992
_refine_ls_wR_factor_ref         0.2517
_reflns_number_gt                2488
_reflns_number_total             5052
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c1cc16264k.txt
_cod_data_source_block           Cs5V14As8O42Br*nH2O
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'multi scan' changed to
'multi-scan' according to the built-in table from CIF Core dictionary
named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_sg_symbol_H-M      C2/c
_cod_original_formula_sum        'As8 Br Cs5 O43.50 V14'
_cod_database_code               7107295
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
As1 As 0.22011(15) -0.04323(13) 0.34816(9) 0.0395(5) Uani 1 1 d .
As2 As 0.00970(15) -0.04424(14) 0.40199(9) 0.0429(6) Uani 1 1 d .
As3 As 0.25700(17) 0.28213(13) 0.26920(11) 0.0483(6) Uani 1 1 d .
As4 As 0.13417(18) 0.28200(15) 0.13321(11) 0.0543(7) Uani 1 1 d .
V1 V 0.1841(2) -0.0087(2) 0.20316(15) 0.0357(8) Uani 1 1 d .
V2 V 0.2811(2) 0.1192(2) 0.31960(15) 0.0388(8) Uani 1 1 d .
V3 V -0.0728(3) 0.1187(2) 0.41036(14) 0.0413(9) Uani 1 1 d .
V4 V 0.1069(3) 0.2475(2) 0.36774(17) 0.0446(9) Uani 1 1 d .
V5 V 0.1505(3) 0.1089(2) 0.41534(15) 0.0431(9) Uani 1 1 d .
V6 V 0.0000 0.3099(3) 0.2500 0.0491(14) Uani 1 2 d S
V7 V 0.2555(2) 0.1289(2) 0.18486(16) 0.0420(9) Uani 1 1 d .
V8 V 0.0000 -0.0730(3) 0.2500 0.0340(10) Uani 1 2 d S
O1 O 0.1411(9) -0.0458(7) 0.2788(5) 0.032(3) Uani 1 1 d .
O2 O 0.1341(10) -0.0712(9) 0.3948(6) 0.043(4) Uani 1 1 d .
O3 O 0.2151(9) 0.0478(8) 0.3634(6) 0.040(3) Uani 1 1 d .
O7 O -0.0453(10) -0.0432(8) 0.3246(6) 0.038(3) Uani 1 1 d .
O8 O 0.0338(10) 0.0453(8) 0.4120(6) 0.039(3) Uani 1 1 d .
O10 O 0.1329(9) 0.2799(9) 0.2888(7) 0.046(4) Uani 1 1 d .
O11 O 0.2129(9) 0.1760(9) 0.3689(6) 0.043(4) Uani 1 1 d .
O12 O 0.2696(9) 0.1897(8) 0.2548(6) 0.040(3) Uani 1 1 d .
O14 O 0.2264(10) 0.3087(9) 0.1928(7) 0.049(4) Uani 1 1 d .
O15 O 0.1683(10) 0.0618(7) 0.1403(6) 0.039(3) Uani 1 1 d .
O16 O 0.2652(9) 0.0619(7) 0.2489(6) 0.034(3) Uani 1 1 d .
O20 O 0.0426(10) 0.1763(10) 0.4117(7) 0.056(4) Uani 1 1 d .
O21 O 0.2618(11) -0.0626(10) 0.1832(7) 0.056(5) Uani 1 1 d .
O22 O 0.1608(11) 0.1883(9) 0.1353(6) 0.051(4) Uani 1 1 d .
O29 O 0.0257(11) 0.2830(9) 0.1700(7) 0.054(4) Uani 1 1 d .
O32 O 0.3954(10) 0.1172(10) 0.3501(7) 0.057(4) Uani 1 1 d .
O34 O 0.3597(11) 0.1287(11) 0.1585(7) 0.060(5) Uani 1 1 d .
O35 O -0.1040(11) 0.1174(11) 0.4753(6) 0.062(5) Uani 1 1 d .
O36 O 0.1549(11) 0.3045(10) 0.4179(7) 0.059(5) Uani 1 1 d .
O37 O 0.0000 -0.1561(12) 0.2500 0.056(6) Uani 1 2 d S
O39 O 0.2110(11) 0.1095(11) 0.4829(7) 0.059(5) Uani 1 1 d .
O46 O 0.0000 0.3879(15) 0.2500 0.083(9) Uani 1 2 d S
Cs2 Cs 0.61108(13) 0.25773(13) 0.04410(8) 0.0768(7) Uani 1 1 d .
Br Br 0.0000 0.1192(2) 0.2500 0.0643(10) Uani 1 2 d S
Cs1 Cs 0.5000 0.04029(14) 0.2500 0.0711(8) Uani 1 2 d S
Cs3 Cs 0.3557(9) 0.0327(8) 0.5769(6) 0.098(5) Uani 0.36 1 d P
Cs5 Cs 0.305(2) -0.041(5) 0.5325(14) 0.15(3) Uani 0.16 1 d P
Cs6 Cs 0.323(4) 0.102(5) 0.013(3) 0.24(4) Uani 0.10 1 d P
Cs7 Cs 0.286(3) 0.026(4) 0.048(2) 0.127(17) Uani 0.16 1 d P
Cs4 Cs 0.3153(16) -0.0148(18) 0.0634(11) 0.093(9) Uani 0.21 1 d P
O47 O -0.0303(16) 0.2412(12) 0.6382(12) 0.067(8) Uani 0.75 1 d P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Br Br -0.2901 2.4595 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 As1 O2 99.3(6) . .
O1 As1 O3 99.4(6) . .
O2 As1 O3 97.8(7) . .
O8 As2 O2 98.0(7) . .
O8 As2 O7 98.9(6) . .
O2 As2 O7 99.5(6) . .
O14 As3 O10 99.3(7) . .
O14 As3 O12 97.0(7) . .
O10 As3 O12 97.9(7) . .
O14 As4 O29 99.9(7) . .
O14 As4 O22 98.9(7) . .
O29 As4 O22 99.8(7) . .
O21 V1 O16 105.6(7) . .
O21 V1 O15 104.4(8) . .
O16 V1 O15 83.6(6) . .
O21 V1 O7 108.7(8) . 2
O16 V1 O7 145.6(6) . 2
O15 V1 O7 90.7(6) . 2
O21 V1 O1 107.4(8) . .
O16 V1 O1 90.5(5) . .
O15 V1 O1 148.0(6) . .
O7 V1 O1 76.6(5) 2 .
O21 V1 V7 108.2(7) . .
O16 V1 V7 41.9(4) . .
O15 V1 V7 41.8(4) . .
O7 V1 V7 125.6(4) 2 .
O1 V1 V7 126.5(4) . .
O21 V1 V8 115.7(7) . .
O16 V1 V8 120.8(4) . .
O15 V1 V8 121.5(4) . .
O7 V1 V8 38.1(4) 2 .
O1 V1 V8 38.7(3) . .
V7 V1 V8 136.13(17) . .
O32 V2 O11 106.5(7) . .
O32 V2 O16 108.8(7) . .
O11 V2 O16 144.7(5) . .
O32 V2 O12 107.2(8) . .
O11 V2 O12 92.9(7) . .
O16 V2 O12 78.1(6) . .
O32 V2 O3 104.3(8) . .
O11 V2 O3 79.1(6) . .
O16 V2 O3 90.9(6) . .
O12 V2 O3 148.4(5) . .
O32 V2 V5 108.9(6) . .
O11 V2 V5 39.0(5) . .
O16 V2 V5 123.9(4) . .
O12 V2 V5 126.2(4) . .
O3 V2 V5 40.1(4) . .
O32 V2 V7 113.0(6) . .
O11 V2 V7 124.6(5) . .
O16 V2 V7 38.5(4) . .
O12 V2 V7 39.6(4) . .
O3 V2 V7 123.8(4) . .
V5 V2 V7 138.09(14) . .
O35 V3 O20 109.1(8) . .
O35 V3 O15 106.9(8) . 2
O20 V3 O15 144.0(6) . 2
O35 V3 O22 105.6(8) . 2
O20 V3 O22 92.1(8) . 2
O15 V3 O22 77.5(6) 2 2
O35 V3 O8 105.3(8) . .
O20 V3 O8 80.2(7) . .
O15 V3 O8 91.1(6) 2 .
O22 V3 O8 149.0(6) 2 .
O35 V3 V5 111.9(6) . .
O20 V3 V5 39.2(6) . .
O15 V3 V5 124.1(4) 2 .
O22 V3 V5 125.5(5) 2 .
O8 V3 V5 41.0(4) . .
O35 V3 V7 110.8(6) . 2
O20 V3 V7 123.2(5) . 2
O15 V3 V7 38.4(4) 2 2
O22 V3 V7 39.1(5) 2 2
O8 V3 V7 124.0(4) . 2
V5 V3 V7 137.22(15) . 2
O36 V4 O20 106.0(8) . .
O36 V4 O10 107.9(8) . .
O20 V4 O10 146.1(7) . .
O36 V4 O29 107.4(8) . 2
O20 V4 O29 91.1(7) . 2
O10 V4 O29 77.1(6) . 2
O36 V4 O11 104.5(7) . .
O20 V4 O11 83.3(7) . .
O10 V4 O11 90.1(6) . .
O29 V4 O11 147.9(6) 2 .
O36 V4 V5 109.0(7) . .
O20 V4 V5 41.7(5) . .
O10 V4 V5 124.9(5) . .
O29 V4 V5 126.5(6) 2 .
O11 V4 V5 41.6(5) . .
O36 V4 V6 114.8(7) . .
O20 V4 V6 121.7(4) . .
O10 V4 V6 38.4(3) . .
O29 V4 V6 38.8(5) 2 .
O11 V4 V6 121.6(4) . .
V5 V4 V6 136.22(18) . .
O39 V5 O11 108.0(8) . .
O39 V5 O20 107.4(7) . .
O11 V5 O20 85.3(7) . .
O39 V5 O3 111.4(7) . .
O11 V5 O3 78.7(6) . .
O20 V5 O3 140.9(6) . .
O39 V5 O8 108.7(8) . .
O11 V5 O8 143.0(5) . .
O20 V5 O8 80.0(7) . .
O3 V5 O8 91.7(6) . .
O39 V5 V4 112.7(7) . .
O11 V5 V4 42.8(4) . .
O20 V5 V4 42.5(5) . .
O3 V5 V4 114.4(5) . .
O8 V5 V4 116.1(4) . .
O39 V5 V3 113.0(6) . .
O11 V5 V3 117.1(4) . .
O20 V5 V3 38.3(5) . .
O3 V5 V3 123.5(4) . .
O8 V5 V3 41.7(4) . .
V4 V5 V3 77.54(14) . .
O39 V5 V2 114.5(6) . .
O11 V5 V2 38.0(4) . .
O20 V5 V2 116.4(5) . .
O3 V5 V2 40.7(5) . .
O8 V5 V2 124.3(4) . .
V4 V5 V2 77.25(15) . .
V3 V5 V2 131.80(15) . .
O46 V6 O10 107.2(5) . .
O46 V6 O10 107.2(5) . 2
O10 V6 O10 145.6(10) . 2
O46 V6 O29 105.3(5) . 2
O10 V6 O29 77.9(6) . 2
O10 V6 O29 93.1(7) 2 2
O46 V6 O29 105.3(5) . .
O10 V6 O29 93.1(7) . .
O10 V6 O29 77.9(6) 2 .
O29 V6 O29 149.5(10) 2 .
O46 V6 V4 113.06(13) . .
O10 V6 V4 38.9(5) . .
O10 V6 V4 123.2(5) 2 .
O29 V6 V4 39.1(4) 2 .
O29 V6 V4 124.7(5) . .
O46 V6 V4 113.06(13) . 2
O10 V6 V4 123.2(5) . 2
O10 V6 V4 38.9(5) 2 2
O29 V6 V4 124.7(5) 2 2
O29 V6 V4 39.1(4) . 2
V4 V6 V4 133.9(3) . 2
O34 V7 O15 107.6(8) . .
O34 V7 O16 108.4(8) . .
O15 V7 O16 84.8(6) . .
O34 V7 O22 108.7(8) . .
O15 V7 O22 78.5(7) . .
O16 V7 O22 142.4(6) . .
O34 V7 O12 108.7(7) . .
O15 V7 O12 143.3(6) . .
O16 V7 O12 78.8(6) . .
O22 V7 O12 94.9(7) . .
O34 V7 V1 112.5(8) . .
O15 V7 V1 42.6(4) . .
O16 V7 V1 42.2(4) . .
O22 V7 V1 115.1(5) . .
O12 V7 V1 115.4(5) . .
O34 V7 V3 113.5(6) . 2
O15 V7 V3 38.5(4) . 2
O16 V7 V3 116.4(4) . 2
O22 V7 V3 40.0(5) . 2
O12 V7 V3 125.6(4) . 2
V1 V7 V3 77.77(13) . 2
O34 V7 V2 113.9(6) . .
O15 V7 V2 116.9(4) . .
O16 V7 V2 38.5(4) . .
O22 V7 V2 125.6(5) . .
O12 V7 V2 40.4(5) . .
V1 V7 V2 77.65(14) . .
V3 V7 V2 132.01(14) 2 .
O37 V8 O7 106.9(4) . .
O37 V8 O7 106.9(4) . 2
O7 V8 O7 146.1(9) . 2
O37 V8 O1 105.3(4) . .
O7 V8 O1 93.0(5) . .
O7 V8 O1 78.1(5) 2 .
O37 V8 O1 105.3(4) . 2
O7 V8 O1 78.1(5) . 2
O7 V8 O1 93.0(5) 2 2
O1 V8 O1 149.3(9) . 2
O37 V8 V1 113.49(11) . .
O7 V8 V1 123.3(4) . .
O7 V8 V1 38.7(4) 2 .
O1 V8 V1 39.6(4) . .
O1 V8 V1 124.1(4) 2 .
O37 V8 V1 113.49(11) . 2
O7 V8 V1 38.7(4) . 2
O7 V8 V1 123.3(4) 2 2
O1 V8 V1 124.1(4) . 2
O1 V8 V1 39.6(4) 2 2
V1 V8 V1 133.0(2) . 2
As1 O1 V8 135.9(7) . .
As1 O1 V1 122.2(6) . .
V8 O1 V1 101.7(5) . .
As1 O2 As2 132.7(9) . .
As1 O3 V5 137.4(8) . .
As1 O3 V2 123.4(7) . .
V5 O3 V2 99.1(7) . .
As2 O7 V8 134.2(8) . .
As2 O7 V1 122.5(7) . 2
V8 O7 V1 103.3(6) . 2
As2 O8 V5 137.5(8) . .
As2 O8 V3 124.6(8) . .
V5 O8 V3 97.2(7) . .
As3 O10 V6 134.9(9) . .
As3 O10 V4 122.3(7) . .
V6 O10 V4 102.7(6) . .
V2 O11 V5 103.0(8) . .
V2 O11 V4 143.7(7) . .
V5 O11 V4 95.6(6) . .
As3 O12 V7 136.9(8) . .
As3 O12 V2 122.3(8) . .
V7 O12 V2 100.0(7) . .
As4 O14 As3 133.2(9) . .
V7 O15 V3 103.1(7) . 2
V7 O15 V1 95.6(6) . .
V3 O15 V1 144.6(8) 2 .
V2 O16 V7 103.0(7) . .
V2 O16 V1 145.5(7) . .
V7 O16 V1 95.9(6) . .
V3 O20 V5 102.5(9) . .
V3 O20 V4 144.9(8) . .
V5 O20 V4 95.8(7) . .
As4 O22 V7 134.7(9) . .
As4 O22 V3 123.7(8) . 2
V7 O22 V3 100.9(8) . 2
As4 O29 V6 134.8(8) . .
As4 O29 V4 123.0(9) . 2
V6 O29 V4 102.1(7) . 2
V5 O39 Cs4 137.6(12) . 6_556
Cs4 Cs3 Cs7 17(4) 6_556 6_556
Cs4 Cs3 Cs5 31(3) 6_556 .
Cs7 Cs3 Cs5 16(2) 6_556 .
Cs4 Cs3 Cs6 44(3) 6_556 6_556
Cs7 Cs3 Cs6 28(3) 6_556 6_556
Cs5 Cs3 Cs6 14.2(18) . 6_556
Cs7 Cs5 Cs4 39(10) 6_556 6_556
Cs7 Cs5 Cs6 147(10) 6_556 6_556
Cs4 Cs5 Cs6 160(4) 6_556 6_556
Cs7 Cs5 Cs3 53(10) 6_556 .
Cs4 Cs5 Cs3 15.6(12) 6_556 .
Cs6 Cs5 Cs3 146(4) 6_556 .
Cs5 Cs6 Cs7 10(3) 6 .
Cs5 Cs6 Cs4 10(2) 6 .
Cs7 Cs6 Cs4 14(2) . .
Cs5 Cs6 Cs3 20(3) 6 6
Cs7 Cs6 Cs3 25(3) . 6
Cs4 Cs6 Cs3 10.8(7) . 6
Cs5 Cs7 Cs4 120(10) 6 .
Cs5 Cs7 Cs3 111(10) 6 6
Cs4 Cs7 Cs3 12(2) . 6
Cs5 Cs7 Cs6 24(10) 6 .
Cs4 Cs7 Cs6 138(5) . .
Cs3 Cs7 Cs6 127(4) 6 .
Cs3 Cs4 Cs7 150(6) 6 .
Cs3 Cs4 Cs5 134(4) 6 6
Cs7 Cs4 Cs5 21(3) . 6
Cs3 Cs4 Cs6 125(4) 6 .
Cs7 Cs4 Cs6 28(4) . .
Cs5 Cs4 Cs6 10(2) 6 .
Cs3 Cs4 O39 104(4) 6 6
Cs7 Cs4 O39 100(4) . 6
Cs5 Cs4 O39 101(3) 6 6
Cs6 Cs4 O39 109.8(15) . 6
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
As1 O1 1.751(11) .
As1 O2 1.764(14) .
As1 O3 1.786(16) .
As2 O8 1.759(15) .
As2 O2 1.784(13) .
As2 O7 1.788(12) .
As3 O14 1.783(15) .
As3 O10 1.793(13) .
As3 O12 1.819(16) .
As4 O14 1.759(15) .
As4 O29 1.788(17) .
As4 O22 1.835(18) .
V1 O21 1.586(14) .
V1 O16 1.936(14) .
V1 O15 1.950(14) .
V1 O7 1.988(13) 2
V1 O1 2.015(13) .
V1 V7 2.866(6) .
V1 V8 3.097(4) .
V2 O32 1.584(13) .
V2 O11 1.895(15) .
V2 O16 1.923(14) .
V2 O12 1.981(15) .
V2 O3 1.981(16) .
V2 V5 2.997(5) .
V2 V7 3.011(5) .
V3 O35 1.586(14) .
V3 O20 1.902(17) .
V3 O15 1.922(14) 2
V3 O22 1.968(17) 2
V3 O8 2.008(15) .
V3 V5 2.994(5) .
V3 V7 3.008(5) 2
V4 O36 1.634(15) .
V4 O20 1.969(18) .
V4 O10 1.970(16) .
V4 O29 1.975(15) 2
V4 O11 1.978(15) .
V4 V5 2.899(6) .
V4 V6 3.061(5) .
V5 O39 1.613(14) .
V5 O11 1.934(16) .
V5 O20 1.938(18) .
V5 O3 1.956(14) .
V5 O8 1.982(15) .
V6 O46 1.50(3) .
V6 O10 1.951(12) .
V6 O10 1.951(12) 2
V6 O29 1.960(18) 2
V6 O29 1.960(18) .
V6 V4 3.061(5) 2
V7 O34 1.607(15) .
V7 O15 1.919(15) .
V7 O16 1.924(14) .
V7 O22 1.933(15) .
V7 O12 1.949(15) .
V7 V3 3.008(5) 2
V8 O37 1.60(2) .
V8 O7 1.963(13) .
V8 O7 1.963(13) 2
V8 O1 1.978(11) .
V8 O1 1.978(11) 2
V8 V1 3.097(4) 2
O7 V1 1.988(13) 2
O15 V3 1.922(14) 2
O22 V3 1.968(17) 2
O29 V4 1.975(15) 2
O39 Cs4 2.79(3) 6_556
Cs3 Cs4 0.67(3) 6_556
Cs3 Cs7 1.54(8) 6_556
Cs3 Cs5 1.81(8) .
Cs3 Cs6 2.95(10) 6_556
Cs5 Cs7 0.54(11) 6_556
Cs5 Cs4 1.28(9) 6_556
Cs5 Cs6 1.28(11) 6_556
Cs6 Cs5 1.28(11) 6
Cs6 Cs7 1.75(12) .
Cs6 Cs4 2.51(10) .
Cs6 Cs3 2.95(10) 6
Cs7 Cs5 0.54(11) 6
Cs7 Cs4 0.92(8) .
Cs7 Cs3 1.54(8) 6
Cs4 Cs3 0.67(3) 6
Cs4 Cs5 1.28(9) 6
Cs4 O39 2.79(3) 6
